- Nano Express
- Open Access
Characterization and Evaluation of Reverse Osmosis Membranes Modified with Ag2O Nanoparticles to Improve Performance
© Al-Hobaib et al. 2015
- Received: 13 July 2015
- Accepted: 17 September 2015
- Published: 29 September 2015
The objective of this work was to prepare and characterize a new and highly efficient modified membrane by in situ interfacial polymerization on porous polysulfone supports. The process used m-phenylenediamine and trimesoyl chloride in hexane, incorporating silver oxide Ag2O nanoparticles of varied concentrations from 0.001 to 0.1 wt%. Ag2O nanoparticles were prepared at different sizes varying between 20 and 50 nm. The modified membranes were characterized by X-ray diffraction (XRD), scanning electron microscopy (SEM), energy-dispersive X-ray spectroscopy (EDX), atomic force microscopy (AFM), transmission electron microscopy (TEM), and contact angle measurement. The results showed a smooth membrane surface and average surface roughness from 31 to 74 nm. Moreover, hydrophilicity improved and the contact angle decreased to 41° at 0.009 wt% silver oxide. The performances of the developed membranes were investigated by measuring permeate fluxes and salt rejection capability by passing NaCl solutions (2000 ppm) through the membranes at 225 psi. The results showed that the flux increased from 26 to 40.5 L/m2 h, while the salt rejection was high, at 99 %, with 0.003 wt% Ag2O nanoparticles.
- Ag2O nanoparticles
- Interfacial polymerization
- RO membrane
- Modified membrane
Water purification technologies are attracting increasing attention, because of gradually increasing shortages of fresh water and lack of access to safe drinking water. Reverse osmosis (RO) is an important membrane technology for water purification through decontamination of industrial effluents and desalination of sea water. Recently, a number of workers have focused on developing high water flux membranes with low processing cost [1–8]. Several methods have already been developed for RO membrane fabrication including phase inversion  and interfacial polymerization (IP) . However, concerted efforts are constantly applied to innovate new efficient supports , polymer types , and tailor polymer structures .
From ancient times, human beings have collected consumable fresh water from rivers, lakes, canals, ponds, and underground aquifers . The sources of fresh water are depleted over time because of several reasons such as growth in population, industrialization, modernization of human societies, and enormous changes in climate. The sources of the fresh water are being contaminated significantly due to agricultural and industrial effluents flowing into lakes, canals, and rivers which are constantly leaking into underground water. These effluents contain many contaminants, such as metals, dyes, pesticides, fertilizers, and biologics, which are harmful to human consumption because of their toxicity [15, 16]. Therefore, human beings are always in search of fresh drinkable water sources for making it available to the consumer. In order to pursue this effort, many physical-chemical methods have been developed and adopted at different times. Some use chemical treatments to remove contaminants from polluted sweet water by adopting various techniques, while others use heat treatment to obtain fresh water through vaporization followed by condensation. These methods are not economically viable, are time consuming, and are environmentally hazardous and unfriendly.
The membrane composition and its subsequent surface chemistry accomplish its interaction with water, thus affecting its wettability. The membrane wettability can be calculated by assessing the contact angle between the membrane surface and a droplet of liquid. Hydrophilic membranes are characterized by the presence of active groups that have the ability to form hydrogen bonds with water and so these membranes have wettability. Generally, higher charge density on a membrane surface is accompanying with higher hydrophilicity of the membrane. Membrane surface morphology also has a considerable effect on flux, fouling as pore size, pore geometry, and pore size distribution particularly at the surface of the membrane .
Surface hydrophilicity augmented when the hydrophilic nanoparticles (NPs) were presented onto the surface of the membrane. Enriched water flux came from the hydrophilic membrane surface. Furthermore, water affinitive surface area improved if the nanoparticle had a higher degree of dispersion and also by increasing membrane hydrophilicity and reduce the cross-linking degree of polyamide thin-film composite membrane by competing with m-phenylenediamine (MPD), which ensued in a great enhancement of water flux. Further, the decrease of the cross-linking degree could also increase salt passage through the membrane [18, 19].
A great number of RO and nanofiltration (NF) membranes with good decontamination performances and permeate fluxes have been developed [20–23]. RO membranes have very high levels of rejection of inorganic solutes such as monovalent ions, hardness components (e.g., calcium, magnesium), and organic matters such as trihalomethane precursor, pesticides, and deodorants at operating pressures of approximately 0.5–6.0 MPa .
An RO membrane is composed of three layers: a bottom layer made of unwoven polyester cloth of thickness 100–200 μm to support the entire membrane, a middle layer consisting of polysulfone (PSF) or polyethersulfone (PES) of thickness 30–50 μm, and a top layer of polyamide (PA) or polyetherimide (PEI), supported by PSF or PES, of average thickness 100–200 nm, which is used to separate solutes from feed water. A PA membrane is prepared on the surface of the middle layer by interfacial polymerization between a diamine moiety of 1,3-phenylenediamine (MPD) in the water phase and an acid chloride moiety of 1,3,5-benzenetricarbonyl trichloride (TMC) in the nonpolar organic phase. An industrial product named FT-30 is one such RO membrane, which has a high level of salt rejection of more than 99 % and fluxes of more than 1 m3/(m2/day) for 2000 ppm NaCl at 1.55 MPa . Thus, many types of RO membranes have been developed.
Kamada et al. developed polyamide RO membranes with controlled surface morphology by interfacial polymerization of water-soaked MPD with TMC in an organic nonpolar hexane medium on polysulfone ultrafiltration supports .
Biofouling and virus penetration are two significant obstacles in water treatment using membrane filtration , because both reduce membrane permeability, increase energy costs, and decrease the lifetime of membranes. To effectively remove viruses, nanofiltration or reverse osmosis should be used with low-pressure membranes having anti-biofouling and antiviral properties. The antibacterial properties of silver are well known, and silver nanoparticles (nano-Ag) are now incorporated into polymer membranes, including RO membranes, as well as in a wide variety of consumer products for microbial control .
In this study, nano-Ag2O was incorporated into RO membranes. Nanosilver oxide incorporation also increases membrane hydrophilicity and reduces the potential for other types of membrane fouling. The objectives of this paper were to prepare and characterize new and highly efficient modified polyamide (PA) membranes incorporating silver oxide (Ag2O) nanoparticles. Ag2O nanoparticles were prepared at different sizes, varying between 20 and 50 nm.
The materials and chemicals which were used in this study are of analytical grade as demonstrated in the following: polysulfone supports (PS-20) were purchased from Sepro, USA; n-hexane (99 %) was purchased from Oxford Laboratory, India; m-phenylenediamine (99 %) (MPD), 1,3,5-benzenetricarbonyl trichloride (TMC), silver nitrate, sodium oleate, triethylene glycol, and n-dodecane (99 %) were purchased from Sigma-Aldrich, USA; n-cyclohexane, n-heptane, and sodium carbonate anhydrous (99 %) were purchased from Scharlau, Spain; ammonium nitrate was purchased from Avonchem Limited, UK; and ultrapure deionized (DI) water was purchased from a Millipore Milli-Q system which was used in all experiments.
Preparation of Ag2O Nanoparticles
Ag2O nanoparticles were prepared by the method as follows: Equimolar quantity of silver nitrate 4.61 g (0.0271 mol) was reacted with 8.25 g (0.0271 mol) sodium oleate to yield silver oleate. The silver oleate thus obtained was added to triethylene glycol and heated to reflux temperature while stirring continuously for about 2 h. The reaction mixture was then centrifuged for 10 min and the supernatant was discarded and dried in an oven at 250 °C for 3 h to a powder, which was finely ground to obtain silver oxide nanoparticles .
Preparation of Polyamide Membranes
Polyamide thin-film composite membranes were prepared by immersing a commercial polysulfone product support (PS-20) in an aqueous solution of MPD (2 v/v%) for 2 min and then the excess MPD solution was removed by pressing the membrane under a rubber roller. The membrane was then immersed in 0.1 % of a TMC and hexane (99 %) solution for 1 min, rinsed with 0.2 % Na2CO3, washed with DI water, and finally stored in a refrigerator ≈4 °C in DI water prior to use.
Synthesis of Polyamide/Silver Oxide Nanocomposite Membranes
The silver oxide-polyamide nanocomposite membranes were synthesized similarly to thin-film composite (TFC) membranes, except that silver oxide nanoparticles were added in the 0.001–0.1 w/v% TMC in n-hexane solution beforehand. Various amounts of Ag2O nanoparticles were dispersed in TMC-n-hexane solution by ultra-sonicating for 60 min at 20 °C. The resultant solution was immediately used for interfacial polymerization (IP) with MPD-soaked PS supports to form the thin-film nanocomposite (TFN) membranes.
Scanning Electron Microscopy (SEM)
The morphology and microstructure of the as-synthesized nanocomposite membrane was examined by scanning electron microscope (SEM; FEI Nova-Nano SEM-600, The Netherlands).
Atomic Force Microscopy (AFM)
The AFM device was a nanosurf scanning probe-optical microscope (Bruker Corporation). Atomic force microscopy was used to analyze the surface morphology and roughness of the prepared membranes. Small squares of the prepared membranes (approximately 1 cm2) were cut and glued on a glass substrate for the analysis.
Contact angle analysis was performed using a Ramé-Hart Model 250 Standard Goniometer/Tensiometer with drop image advanced software (Ramé-Hart Instrument Co., Succasunna, NJ). A water droplet was placed on a dry, flat homogeneous membrane surface, and the contact angle between the water and membrane was measured until no further change was observed. The average contact angle for distilled water was determined in a series of eight measurements for each of the different membrane surfaces.
Cross-Flow (Flux and Salt Rejection)
where C p and C f are the salt concentrations in the permeate and feed streams, respectively.
The synthesized silver oxide nanoparticles were characterized by SEM, transmission electron microscopy (TEM), energy-dispersive spectroscopy (EDX), and X-ray diffraction (XRD) as follows.
It can be observed that contact angle significantly decreased with increased silver oxide content in the membranes. For example, the presence of a silver content of 0.003 wt% in the membrane dropped the contact angle from 94° ± 1.8° to 45° ± 0.7°. Contact angles of the membranes did not change/decrease markedly above 0.01 wt% silver loading. Additionally, the hydrophilicity did not change significantly, despite the increasing content of Ag2O nanoparticles. Our results are in agreement with those obtained by other researchers . It is known that there is a strong correlation between the geometry/stereochemistry of water at the solid-liquid interface and the hydrophilicity of the solid surface [32, 33]. Rearrangement of interfacial water molecules can increase hydrophilicity, thus improving water’s ability to form hydrogen bonds and, in turn, producing stronger interactions between water and the solid phase in the polymer matrix, i.e., the TFC surface.
A large amount of embedded spherical Ag2O nanoparticles could have been exposed on the membrane surface. The hydrophilic nature of the silver nanoparticles would increase the hydrophilic character of the membrane surface and would also help water molecules to adhere to the Ag2O nanoparticles, through capillary effects . This is consistent with the result of Jeong et al. , who observed that the contact angle of membrane surface decreased with increased zeolite content and attributed this to the super-hydrophilic property of the zeolite.
Second, silver oxide nanoparticles may hydrate and release heat when contacting with MPD aqueous solution . This process may affect the IP reaction between MPD and TMC and, subsequently, may change the matrix of the PS support. If a large number of acyl chloride groups of TMC remained on the membrane surface without reacting with the amine groups of MPD, the hydrolysis of acyl chloride could generate carboxylic acid functional groups, which may lead to increased hydrophilicity . It is known that the hydrophilic nature of Ag2O nanoparticles can significantly improve the overall hydrophilicity of membranes, thereby creating favorable conditions for improved water flux and antifouling. It is well understood that the morphological structure and the hydrophilicity of the membrane are the two main factors that govern the filtration properties of membranes and those of TFC membranes .
Summary of membrane characteristics of present study
Salt rejection %
Flux (L/m2 h)
Constant at 2 %
Constant at 0.1 %
99 ± 0.1
30.43 ± 2.1
99 ± 0.1
40.43 ± 3.0
98 ± 0.3
29.57 ± 1.9
99 ± 0.1
26.64 ± 2.2
98 ± 0.2
30.14 ± 2.1
99 ± 0.1
30.83 ± 2.9
94 ± 0.7
24.33 ± 1.7
98 ± 0.2
21.50 ± 2.2
97 ± 0.9
15.43 ± 2.9
99 ± 0.1
18.90 ± 2.1
Both permeate flux and salt rejection ability depend on the polyamide layer density, which is related to cross-linking density . The polymer density across the barrier layer is not uniform . The core layer (near the original MPD/TMC interface) is the most dense region, and the polymer density decreases gradually as the polymer grows further into the organic phase [41, 42]. In many applications of interfacial polymerization using MPD and TMC, the initial amine concentration is much higher than the acyl chloride concentration. Whether the amine concentration is decreased or the acyl chloride concentration is increased, this results in a more dense polyamide layer, compared with those prepared using higher amine/acid chloride molar ratios . An increase in density or in thickness of the MPD/TMC barrier layer would increase the mass transfer resistance of the resulting membrane, thereby reducing permeate flux. Thus, varying the initial concentration of monomers can influence the membrane’s water and salt transport properties.
Salt passage was found to be relatively insensitive to changes in MPD concentration. This suggests the formation of defect-free membranes in all cases. Maximum permeate flux was exhibited near 2 w/v% MPD. As the MPD concentration was increased, the driving force for MPD diffusion into the organic phase increased. Increased MPD concentration could, therefore, increase the barrier layer thickness and, thus, causes a lower permeate flux. As MPD concentration decreased, layer thickness was expected to decrease, which would tend to increase flux, but the resulting layer was also expected to become more dense as the molar ratio of amine/acyl chloride approached unity, which would lower flux [41, 44].
Figure 10 illustrates the influence of TMC concentration in the organic phase on permeate flux and salt passage at a constant MPD concentration of 2 w/v% in the aqueous phase, which was observed in Fig. 9 to be near the optimum flux value. Interfacial polymerization is typically MPD diffusion-controlled during growth of the polyamide layer. If TMC concentration is increased, the amine/acyl chloride molar ratio will decrease. This will, in turn, increase film density, causing a lower permeate flux [41, 44]. However, a decrease in permeate flux was also observed at the lowest TMC concentration of <0.1 %. Thus, the interfacial polymerization reaction is also reported to be TMC diffusion-limited . A low concentration of acyl chloride groups in the reaction zone may allow the polyamide film to grow thicker, which would decrease flux .
Summary of membrane characteristics from previous studies
Modified membrane properties
Flux (L/m2 h)
Enhanced surface hydrophilicity, increase roughness
MgTiO3 in TMC/hexane
Smoother, hydrophilic, and negatively charged surfaces
NaA in TMC/hexane
Silica particle interacting well with the polyamide
Silica in MPD/water
Tunable pore radius and higher thermal stability
Silica in MPD/water
Higher anti-biofouling effect
Silver in BTC
The neat TFC membrane was dipped in the transparent TiO2 colloidal solution
Higher photocatalytic bactericidal efficiency under UV light
Enhanced surface hydrophilicity
TiO2 in TMC and HCFC
Increase roughness and contact angle
NaY in TMC/hexane
Enhanced surface hydrophilicity
Al2O3 in TMC/hexane
Silver oxide nanoparticles were embedded into the polyamide membrane through an interfacial polymerization process between MPD and TMC. EDX and SEM confirmed the formation of polyamide membranes embedded with silver oxide nanoparticles. EDX quantitative analysis confirmed the presence of silver oxide in polyamide components. Water flux and salt rejection performances revealed that the nanocomposite membrane was superior to the native (unmodified) membrane. Moreover, permeate flux was improved (from 26 to 40.5 L/m2 h), while salt rejection performances remained within 2 %.
The authors are grateful to the King Abdulaziz City for Science and Technology, Riyadh, Saudi Arabia, for the financial support of this work and the facilities in its labs. This work was supported by King Saud University, Deanship of Scientific Research, College of Science, Research Center.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Kim SH, Kwak S-Y, Sohn B-H, Park TH. Design of TiO2 nanoparticle self-assembled aromatic polyamide thin-film-composite (TFC) membrane as an approach to solve biofouling problem. J Membr Sci. 2003;211(1):157–65.View ArticleGoogle Scholar
- Ghosh AK, Hoek EM. Impacts of support membrane structure and chemistry on polyamide–polysulfone interfacial composite membranes. J Membr Sci. 2009;336(1):140–8.View ArticleGoogle Scholar
- Van Voorthuizen EM, Zwijnenburg A, Wessling M. Nutrient removal by NF and RO membranes in a decentralized sanitation system. Water Res. 2005;39(15):3657–67.View ArticleGoogle Scholar
- Peng X, Jin J, Nakamura Y, Ohno T, Ichinose I. Ultrafast permeation of water through protein-based membranes. Nat Nanotech. 2009;4(6):353–7.View ArticleGoogle Scholar
- Zhou M, Nemade PR, Lu X, Zeng X, Hatakeyama ES, Noble RD, et al. New type of membrane material for water desalination based on a cross-linked bicontinuous cubic lyotropic liquid crystal assembly. J Am Chem Soc. 2007;129(31):9574–5.View ArticleGoogle Scholar
- Tsuru T. Inorganic porous membranes for liquid phase separation. Sep Purif Rev. 2001;30(2):191–220.View ArticleGoogle Scholar
- AL-Sheetan KM, Shaik MR, Al-Hobaib AS, Alandis NM. Characterization and evaluation of the improved performance of modified reverse osmosis membranes by incorporation of various organic modifiers and SnO2 nanoparticles. J Nanomater. 2015;Article ID 363175:1–11.View ArticleGoogle Scholar
- Suk M, Raghunathan A, Aluru N. Fast reverse osmosis using boron nitride and carbon nanotubes. Appl Phy Lett. 2008;92(13):133120.View ArticleGoogle Scholar
- Petersen RJ. Composite reverse osmosis and nanofiltration membranes. J Membr Sci. 1993;83(1):81–150.View ArticleGoogle Scholar
- Rao AP, Desai N, Rangarajan R. Interfacially synthesized thin film composite RO membranes for seawater desalination. J Membr Sci. 1997;124(2):263–72.View ArticleGoogle Scholar
- Yoon K, Hsiao BS, Chu B. High flux nanofiltration membranes based on interfacially polymerized polyamide barrier layer on polyacrylonitrile nanofibrous scaffolds. J Membr Sci. 2009;326(2):484–92.View ArticleGoogle Scholar
- Li L, Zhang S, Zhang X. Preparation and characterization of poly (piperazineamide) composite nanofiltration membrane by interfacial polymerization of 3, 3′, 5, 5′-biphenyl tetraacyl chloride and piperazine. J Membr Sci. 2009;335(1):133–9.View ArticleGoogle Scholar
- Tarboush BJA, Rana D, Matsuura T, Arafat H, Narbaitz R. Preparation of thin-film-composite polyamide membranes for desalination using novel hydrophilic surface modifying macromolecules. J Membr Sci. 2008;325(1):166–75.View ArticleGoogle Scholar
- Jenerette GD, Larsen L. A global perspective on changing sustainable urban water supplies. Global Planet Change. 2006;50(3):202–11.View ArticleGoogle Scholar
- Kim I-C, Lee K-H. Dyeing process wastewater treatment using fouling resistant nanofiltration and reverse osmosis membranes. Desalination. 2006;192(1):246–51.View ArticleGoogle Scholar
- Ju H, McCloskey BD, Sagle AC, Wu Y-H, Kusuma VA, Freeman BD. Crosslinked poly (ethylene oxide) fouling resistant coating materials for oil/water separation. J Membr Sci. 2008;307(2):260–7.View ArticleGoogle Scholar
- Kim SG, Hyeon DH, Chun JH, Chun B-H, Kim SH. Nanocomposite poly (arylene ether sulfone) reverse osmosis membrane containing functional zeolite nanoparticles for seawater desalination. J Membr Sci. 2013;443:10–8.View ArticleGoogle Scholar
- Dong H, Zhao L, Zhang L, Chen H, Gao C, Ho WW. High-flux reverse osmosis membranes incorporated with NaY zeolite nanoparticles for brackish water desalination. J Membr Sci. 2015;476:373–83.View ArticleGoogle Scholar
- Zhao L, Ho WW. Novel reverse osmosis membranes incorporated with a hydrophilic additive for seawater desalination. J Membr Sci. 2014;455:44–54.View ArticleGoogle Scholar
- Tang CY, Kwon Y-N, Leckie JO. Effect of membrane chemistry and coating layer on physiochemical properties of thin film composite polyamide RO and NF membranes: I. FTIR and XPS characterization of polyamide and coating layer chemistry. Desalination. 2009;242(1):149–67.View ArticleGoogle Scholar
- Baker RW. Membrane Technology. Kirk- Othmer encyclopedia of Chemical technology. 2000; DOI: 10.1002/0471238961.1305130202011105.a01.
- Kurihara M, Hanakawa M. Mega-ton Water System: Japanese national research and development project on seawater desalination and wastewater reclamation. Desalination. 2013;308:131–7.View ArticleGoogle Scholar
- Xie W, Geise GM, Freeman BD, Lee H-S, Byun G, McGrath JE. Polyamide interfacial composite membranes prepared from m-phenylene diamine, trimesoyl chloride and a new disulfonated diamine. J Membr Sci. 2012;403:152–61.View ArticleGoogle Scholar
- Vrijenhoek EM, Hong S, Elimelech M. Influence of membrane surface properties on initial rate of colloidal fouling of reverse osmosis and nanofiltration membranes. J Membr Sci. 2001;188(1):115–28.View ArticleGoogle Scholar
- Cadotte JE. Interfacially synthesized reverse osmosis membrane. Google Patents. 1981.Google Scholar
- Kamada T, Ohara T, Shintani T, Tsuru T. Optimizing the preparation of multi-layered polyamide membrane via the addition of a co-solvent. J Membr Sci. 2014;453:489–97.View ArticleGoogle Scholar
- Zodrow K, Brunet L, Mahendra S, Li D, Zhang A, Li Q, et al. Polysulfone ultrafiltration membranes impregnated with silver nanoparticles show improved biofouling resistance and virus removal. Water Res. 2009;43(3):715–23.View ArticleGoogle Scholar
- Siddiqui MRH, Adil S, Assal M, Ali R, Al-Warthan A. Synthesis and characterization of silver oxide and silver chloride nanoparticles with high thermal stability. Asian J Chem. 2013;25(6):3405–9.Google Scholar
- Lind ML, Eumine Suk D, Nguyen T-V, Hoek EM. Tailoring the structure of thin film nanocomposite membranes to achieve seawater RO membrane performance. Environ Sci Technol. 2010;44(21):8230–5.View ArticleGoogle Scholar
- Khan M, Khan M, Adil SF, Tahir MN, Tremel W, Alkhathlan HZ, et al. Green synthesis of silver nanoparticles mediated by Pulicaria glutinosa extract. Int J Nanomedicine. 2013;8:1507–16.Google Scholar
- Yin J, Kim E-S, Yang J, Deng B. Fabrication of a novel thin-film nanocomposite (TFN) membrane containing MCM-41 silica nanoparticles (NPs) for water purification. J Membr Sci. 2012;423:238–46.View ArticleGoogle Scholar
- Hurwitz G, Guillen GR, Hoek EM. Probing polyamide membrane surface charge, zeta potential, wettability, and hydrophilicity with contact angle measurements. J Membr Sci. 2010;349(1):349–57.View ArticleGoogle Scholar
- Du Q, Freysz E, Shen YR. Surface vibrational spectroscopic studies of hydrogen bonding and hydrophobicity. Science. 1994;264(5160):826–8.View ArticleGoogle Scholar
- Li J-H, Xu Y-Y, Zhu L-P, Wang J-H, Du C-H. Fabrication and characterization of a novel TiO2 nanoparticle self-assembly membrane with improved fouling resistance. J Membr Sci. 2009;326(2):659–66.View ArticleGoogle Scholar
- Jeong B-H, Hoek EM, Yan Y, Subramani A, Huang X, Hurwitz G, et al. Interfacial polymerization of thin film nanocomposites: a new concept for reverse osmosis membranes. J Membr Sci. 2007;294(1):1–7.View ArticleGoogle Scholar
- Lind ML, Ghosh AK, Jawor A, Huang X, Hou W, Yang Y, et al. Influence of zeolite crystal size on zeolite-polyamide thin film nanocomposite membranes. Langmuir. 2009;25(17):10139–45.View ArticleGoogle Scholar
- Kim C, Kim J, Roh I, Kim J. The changes of membrane performance with polyamide molecular structure in the reverse osmosis process. J Membr Sci. 2000;165(2):189–99.View ArticleGoogle Scholar
- Wu H, Tang B, Wu P. Novel ultrafiltration membranes prepared from a multi-walled carbon nanotubes/polymer composite. J Membr Sci. 2010;362(1):374–83.View ArticleGoogle Scholar
- Song Y, Sun P, Henry LL, Sun B. Mechanisms of structure and performance controlled thin film composite membrane formation via interfacial polymerization process. J Membr Sci. 2005;251(1):67–79.View ArticleGoogle Scholar
- Mitchell GE, Mickols B, Hernandez-Cruz D, Hitchcock A. Unexpected new phase detected in FT30 type reverse osmosis membranes using scanning transmission X-ray microscopy. Polymer. 2011;52(18):3956–62.View ArticleGoogle Scholar
- Freger V. Nanoscale heterogeneity of polyamide membranes formed by interfacial polymerization. Langmuir. 2003;19(11):4791–7.View ArticleGoogle Scholar
- Pacheco FA, Pinnau I, Reinhard M, Leckie JO. Characterization of isolated polyamide thin films of RO and NF membranes using novel TEM techniques. J Membr Sci. 2010;358(1):51–9.View ArticleGoogle Scholar
- Berezkin AV, Khokhlov AR. Mathematical modeling of interfacial polycondensation. J Polym Sci Part B: Polym Phy. 2006;44(18):2698–724.View ArticleGoogle Scholar
- Freger V, Srebnik S. Mathematical model of charge and density distributions in interfacial polymerization of thin films. J Appl Polym Sci. 2003;88(5):1162–9.View ArticleGoogle Scholar
- Chai G-Y, Krantz WB. Formation and characterization of polyamide membranes via interfacial polymerization. J Membr Sci. 1994;93(2):175–92.View ArticleGoogle Scholar
- AL-Hobaib A, El Ghoul J, El Mir L. Fabrication of polyamide membrane reached by MgTiO3 nanoparticles for ground water purification. Desalin Water Treat. 2015; 1–10. (ahead-of-print)Google Scholar
- Domingues SH, Salvatierra RV, Oliveira MM, Zarbin AJ. Transparent and conductive thin films of graphene/polyaniline nanocomposites prepared through interfacial polymerization. Chem Commun. 2011;47(9):2592–4.View ArticleGoogle Scholar
- Singh PS, Aswal VK. Characterization of physical structure of silica nanoparticles encapsulated in polymeric structure of polyamide films. J Colloid Interface Sci. 2008;326(1):176–85.View ArticleGoogle Scholar
- Jadav GL, Singh PS. Synthesis of novel silica-polyamide nanocomposite membrane with enhanced properties. J Membr Sci. 2009;328(1):257–67.View ArticleGoogle Scholar
- Lee SY, Kim HJ, Patel R, Im SJ, Kim JH, Min BR. Silver nanoparticles immobilized on thin film composite polyamide membrane: characterization, nanofiltration, antifouling properties. Polym Advan Technol. 2007;18(7):562–8.View ArticleGoogle Scholar
- Kwak S-Y, Kim SH, Kim SS. Hybrid organic/inorganic reverse osmosis (RO) membrane for bactericidal anti-fouling. 1. Preparation and characterization of TiO2 nanoparticle self-assembled aromatic polyamide thin-film-composite (TFC) membrane. Environ Sci Technol. 2001;35(11):2388–94.View ArticleGoogle Scholar
- Lee HS, Im SJ, Kim JH, Kim HJ, Kim JP, Min BR. Polyamide thin-film nanofiltration membranes containing TiO2 nanoparticles. Desalination. 2008;219(1):48–56.View ArticleGoogle Scholar
- Ma N, Wei J, Liao R, Tang CY. Zeolite-polyamide thin film nanocomposite membranes: towards enhanced performance for forward osmosis. J Membr Sci. 2012;405:149–57.View ArticleGoogle Scholar
- Saleh TA, Gupta VK. Synthesis and characterization of alumina nano-particles polyamide membrane with enhanced flux rejection performance. Sep Purif Technol. 2012;89:245–51.View ArticleGoogle Scholar